#------------------------------------------------------------------------------
#$Date: 2024-01-06 21:08:10 +0200 (Sat, 06 Jan 2024) $
#$Revision: 288919 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/07/1570710.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1570710
loop_
_publ_author_name
'Kurig, Sophia'
'Ketter, Fabian'
'Frommelius, Anne'
'Hakala, B. Viliam'
'van Leusen, Jan'
'Friese, Karen'
'Dronskowski, Richard'
_publ_section_title
;
 Exploring the Structure and Properties of VwSeyTe2−y Mixed
 Crystals in the VTe2--VSe2 System
;
_journal_issue                   12
_journal_name_full               Inorganics
_journal_page_first              481
_journal_paper_doi               10.3390/inorganics11120481
_journal_volume                  11
_journal_year                    2023
_chemical_formula_sum            'Se0.72 Te1.28 V1.13'
_chemical_formula_weight         277.74
_space_group_crystal_system      trigonal
_space_group_IT_number           164
_space_group_name_Hall           '-P 3 2"'
_space_group_name_H-M_alt        'P -3 m 1'
_audit_creation_method           SHELXL-2018/1
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.6259(14)
_cell_length_b                   3.6259(14)
_cell_length_c                   6.290(2)
_cell_measurement_reflns_used    582
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.770
_cell_measurement_theta_min      3.239
_cell_volume                     71.62(5)
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'Bruker APEX CCD'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0247
_diffrn_reflns_av_unetI/netI     0.0131
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.982
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            1049
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.982
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.402
_diffrn_reflns_theta_min         3.239
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    25.541
_exptl_absorpt_correction_T_max  0.7460
_exptl_absorpt_correction_T_min  0.5243
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABAS, R. H. Blessing, Acta Crystallogr. A 1995, 51, 33'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.441
_exptl_crystal_description       hexagonal
_exptl_crystal_F_000             117
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.04
_refine_diff_density_max         1.454
_refine_diff_density_min         -1.198
_refine_diff_density_rms         0.218
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.208
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     11
_refine_ls_number_reflns         108
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.208
_refine_ls_R_factor_all          0.0222
_refine_ls_R_factor_gt           0.0204
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0240P)²+0.2441P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0482
_refine_ls_wR_factor_ref         0.0491
_reflns_Friedel_coverage         0.000
_reflns_number_gt                103
_reflns_number_total             108
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            V1.13Se0.72Te1.28_final.cif
_cod_data_source_block           shelx
_cod_original_cell_volume        71.62(6)
_cod_database_code               1570710
_shelx_shelxl_version_number     2018/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
V1 V 0.000000 0.000000 0.000000 0.0582(13) Uani 1 12 d S T P . .
V2 V 0.000000 0.000000 0.500000 0.028(6) Uani 0.128(11) 12 d S T . . .
Se Se 0.333333 0.666667 0.235(3) 0.0212(7) Uani 0.36(3) 6 d S T P . .
Te Te 0.333333 0.666667 0.2652(11) 0.0212(7) Uani 0.64(3) 6 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Se V1 Se 90.1(5) 7 7_665 ?
Se V1 Se 89.9(5) 7 1_445 ?
Se V1 Se 180.0 7_665 1_445 ?
Se V1 Se 180.0 7 . ?
Se V1 Se 89.9(5) 7_665 . ?
Se V1 Se 90.1(5) 1_445 . ?
Se V1 Se 90.1(5) 7 7_565 ?
Se V1 Se 90.1(5) 7_665 7_565 ?
Se V1 Se 89.9(5) 1_445 7_565 ?
Se V1 Se 89.9(5) . 7_565 ?
Se V1 Se 89.9(5) 7 1_545 ?
Se V1 Se 89.9(5) 7_665 1_545 ?
Se V1 Se 90.1(5) 1_445 1_545 ?
Se V1 Se 90.1(5) . 1_545 ?
Se V1 Se 180.0 7_565 1_545 ?
Se V1 Te 3.3(4) 7 7 ?
Se V1 Te 87.7(2) 7_665 7 ?
Se V1 Te 92.3(2) 1_445 7 ?
Se V1 Te 176.7(4) . 7 ?
Se V1 Te 87.7(2) 7_565 7 ?
Se V1 Te 92.3(2) 1_545 7 ?
Se V1 Te 87.7(2) 7 7_665 ?
Se V1 Te 3.3(4) 7_665 7_665 ?
Se V1 Te 176.7(4) 1_445 7_665 ?
Se V1 Te 92.3(2) . 7_665 ?
Se V1 Te 87.7(2) 7_565 7_665 ?
Se V1 Te 92.3(2) 1_545 7_665 ?
Te V1 Te 85.27(18) 7 7_665 ?
Se V1 Te 92.3(2) 7 1_445 ?
Se V1 Te 176.7(4) 7_665 1_445 ?
Se V1 Te 3.3(4) 1_445 1_445 ?
Se V1 Te 87.7(2) . 1_445 ?
Se V1 Te 92.3(2) 7_565 1_445 ?
Se V1 Te 87.7(2) 1_545 1_445 ?
Te V1 Te 94.73(18) 7 1_445 ?
Te V1 Te 180.0 7_665 1_445 ?
Se V1 Te 176.7(4) 7 . ?
Se V1 Te 92.3(2) 7_665 . ?
Se V1 Te 87.7(2) 1_445 . ?
Se V1 Te 3.3(4) . . ?
Se V1 Te 92.3(2) 7_565 . ?
Se V1 Te 87.7(2) 1_545 . ?
Te V1 Te 180.0(2) 7 . ?
Te V1 Te 94.73(18) 7_665 . ?
Te V1 Te 85.27(18) 1_445 . ?
Se V1 Te 92.3(2) 7 1_545 ?
Se V1 Te 92.3(2) 7_665 1_545 ?
Se V1 Te 87.7(2) 1_445 1_545 ?
Se V1 Te 87.7(2) . 1_545 ?
Se V1 Te 176.7(4) 7_565 1_545 ?
Se V1 Te 3.3(4) 1_545 1_545 ?
Te V1 Te 94.73(18) 7 1_545 ?
Te V1 Te 94.73(18) 7_665 1_545 ?
Te V1 Te 85.27(18) 1_445 1_545 ?
Te V1 Te 85.27(18) . 1_545 ?
Se V1 Te 87.7(2) 7 7_565 ?
Se V1 Te 87.7(2) 7_665 7_565 ?
Se V1 Te 92.3(2) 1_445 7_565 ?
Se V1 Te 92.3(2) . 7_565 ?
Se V1 Te 3.3(4) 7_565 7_565 ?
Se V1 Te 176.7(4) 1_545 7_565 ?
Te V1 Te 85.27(18) 7 7_565 ?
Te V1 Te 85.27(18) 7_665 7_565 ?
Te V1 Te 94.73(18) 1_445 7_565 ?
Te V1 Te 94.73(18) . 7_565 ?
Te V1 Te 180.0 1_545 7_565 ?
Te V2 Te 180.0 7_666 1_445 ?
Te V2 Te 90.08(19) 7_666 7_556 ?
Te V2 Te 89.92(19) 1_445 7_556 ?
Te V2 Te 89.92(19) 7_666 . ?
Te V2 Te 90.08(19) 1_445 . ?
Te V2 Te 180.0 7_556 . ?
Te V2 Te 90.08(19) 7_666 7_566 ?
Te V2 Te 89.92(19) 1_445 7_566 ?
Te V2 Te 90.08(19) 7_556 7_566 ?
Te V2 Te 89.92(19) . 7_566 ?
Te V2 Te 89.92(19) 7_666 1_545 ?
Te V2 Te 90.08(19) 1_445 1_545 ?
Te V2 Te 89.92(19) 7_556 1_545 ?
Te V2 Te 90.08(19) . 1_545 ?
Te V2 Te 180.0 7_566 1_545 ?
Te V2 Se 176.7(4) 7_666 1_445 ?
Te V2 Se 3.3(4) 1_445 1_445 ?
Te V2 Se 92.3(2) 7_556 1_445 ?
Te V2 Se 87.7(2) . 1_445 ?
Te V2 Se 92.3(2) 7_566 1_445 ?
Te V2 Se 87.7(2) 1_545 1_445 ?
Te V2 Se 3.3(4) 7_666 7_666 ?
Te V2 Se 176.7(4) 1_445 7_666 ?
Te V2 Se 87.7(2) 7_556 7_666 ?
Te V2 Se 92.3(2) . 7_666 ?
Te V2 Se 87.7(2) 7_566 7_666 ?
Te V2 Se 92.3(2) 1_545 7_666 ?
Se V2 Se 180.0(6) 1_445 7_666 ?
Te V2 Se 92.3(2) 7_666 . ?
Te V2 Se 87.7(2) 1_445 . ?
Te V2 Se 176.7(4) 7_556 . ?
Te V2 Se 3.3(4) . . ?
Te V2 Se 92.3(2) 7_566 . ?
Te V2 Se 87.7(2) 1_545 . ?
Se V2 Se 85.3(5) 1_445 . ?
Se V2 Se 94.7(5) 7_666 . ?
Te V2 Se 87.7(2) 7_666 7_556 ?
Te V2 Se 92.3(2) 1_445 7_556 ?
Te V2 Se 3.3(4) 7_556 7_556 ?
Te V2 Se 176.7(4) . 7_556 ?
Te V2 Se 87.7(2) 7_566 7_556 ?
Te V2 Se 92.3(2) 1_545 7_556 ?
Se V2 Se 94.7(5) 1_445 7_556 ?
Se V2 Se 85.3(5) 7_666 7_556 ?
Se V2 Se 180.0 . 7_556 ?
Te V2 Se 87.7(2) 7_666 7_566 ?
Te V2 Se 92.3(2) 1_445 7_566 ?
Te V2 Se 87.7(2) 7_556 7_566 ?
Te V2 Se 92.3(2) . 7_566 ?
Te V2 Se 3.3(4) 7_566 7_566 ?
Te V2 Se 176.7(4) 1_545 7_566 ?
Se V2 Se 94.7(5) 1_445 7_566 ?
Se V2 Se 85.3(5) 7_666 7_566 ?
Se V2 Se 94.7(5) . 7_566 ?
Se V2 Se 85.3(5) 7_556 7_566 ?
Te V2 Se 92.3(2) 7_666 1_545 ?
Te V2 Se 87.7(2) 1_445 1_545 ?
Te V2 Se 92.3(2) 7_556 1_545 ?
Te V2 Se 87.7(2) . 1_545 ?
Te V2 Se 176.7(4) 7_566 1_545 ?
Te V2 Se 3.3(4) 1_545 1_545 ?
Se V2 Se 85.3(5) 1_445 1_545 ?
Se V2 Se 94.7(5) 7_666 1_545 ?
Se V2 Se 85.3(5) . 1_545 ?
Se V2 Se 94.7(5) 7_556 1_545 ?
Se V2 Se 180.0 7_566 1_545 ?
V1 Se V1 90.1(5) 1_565 . ?
V1 Se V1 90.1(5) 1_565 1_665 ?
V1 Se V1 90.1(5) . 1_665 ?
V1 Se V2 132.75(5) 1_565 1_665 ?
V1 Se V2 132.75(5) . 1_665 ?
V1 Se V2 73.76(4) 1_665 1_665 ?
V1 Se V2 73.76(4) 1_565 1_565 ?
V1 Se V2 132.75(5) . 1_565 ?
V1 Se V2 132.75(5) 1_665 1_565 ?
V2 Se V2 85.3(5) 1_665 1_565 ?
V1 Se V2 132.75(5) 1_565 . ?
V1 Se V2 73.76(4) . . ?
V1 Se V2 132.75(5) 1_665 . ?
V2 Se V2 85.3(5) 1_665 . ?
V2 Se V2 85.3(5) 1_565 . ?
V2 Te V2 90.08(19) 1_665 1_565 ?
V2 Te V2 90.08(19) 1_665 . ?
V2 Te V2 90.08(19) 1_565 . ?
V2 Te V1 132.75(2) 1_665 . ?
V2 Te V1 132.75(2) 1_565 . ?
V2 Te V1 73.76(3) . . ?
V2 Te V1 132.75(2) 1_665 1_565 ?
V2 Te V1 73.76(3) 1_565 1_565 ?
V2 Te V1 132.75(2) . 1_565 ?
V1 Te V1 85.27(18) . 1_565 ?
V2 Te V1 73.76(3) 1_665 1_665 ?
V2 Te V1 132.75(2) 1_565 1_665 ?
V2 Te V1 132.75(2) . 1_665 ?
V1 Te V1 85.27(18) . 1_665 ?
V1 Te V1 85.27(18) 1_565 1_665 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
V1 Se 2.562(11) 7 ?
V1 Se 2.562(11) 7_665 ?
V1 Se 2.562(11) 1_445 ?
V1 Se 2.562(11) . ?
V1 Se 2.562(11) 7_565 ?
V1 Se 2.562(11) 1_545 ?
V1 Te 2.677(5) 7 ?
V1 Te 2.677(5) 7_665 ?
V1 Te 2.677(5) 1_445 ?
V1 Te 2.677(5) . ?
V1 Te 2.677(5) 1_545 ?
V1 Te 2.677(5) 7_565 ?
V2 Te 2.562(4) 7_666 ?
V2 Te 2.562(4) 1_445 ?
V2 Te 2.562(4) 7_556 ?
V2 Te 2.562(4) . ?
V2 Te 2.562(4) 7_566 ?
V2 Te 2.562(4) 1_545 ?
V2 Se 2.677(12) 1_445 ?
V2 Se 2.677(12) 7_666 ?
V2 Se 2.677(12) . ?
V2 Se 2.677(12) 7_556 ?
V2 Se 2.677(12) 7_566 ?
V2 Se 2.677(12) 1_545 ?
